Esterification of Benzyl Alcohol with Acetic Acid over
Desy Tri Kusumaningtyas1, Didik Prasetyoko1*, S. Suprapto1, Sugeng Triwahyono2, Aishah Abdul Jalil2, Afifah Rosidah1
1Department of Chemistry, Institut Teknologi Sepuluh Nopember, Surabaya 60111, Indonesia 2Ibnu Sina Institute for Fundamental Science Studies, Universiti Teknologi Malaysia,
Skudai, Johor Bahru 81310, Malaysia
Bulletin of Chemical Reaction Engineering & Catalysis, 12 (2), 2017, 243-250
In this study, the performance of mesoporous ZSM-5 has been studied on the esterification of acetic acid (AA) with benzyl alcohol (BA). The mesoporous ZSM-5 catalyst has been synthesized with the variation of aging time i.e. 6, 12, and 24 hours at the same temperature, 70 °C. The cation exchange of Na-ZSM-5 to H-ZSM-5 was performed before the catalytic activity test. The acidity type and amount of solids were determined by FT-IR spectroscopy using pyridine as a probe molecule. The characterization by pyridine adsorption showed that at a higher mesoporous surface area, the number of Lewis acid was increased. The highest mesoporous surface area, Lewis, and Brönsted acid sites were obtained by sam-ple which has the lowest crystallinity, i.e. 255.78 m2/g, 0.2732 mmol/g, and 0.20612 mmol/g, respec-tively. Influence of mesoporous volume was studied on the catalytic activity of the mesoporous ZSM-5 in the esterification reaction. Conversion of acetic acid in the esterification reaction for samples of HZ-6, HZ-12, and HZ-24 were obtained by titration methods, i.e. 39.59, 36.39, and 32.90 %, respec-tively. Hence, the reaction temperature of 393 K, molar ratio 1:4 (AA:BA) and catalyst loading 5 % were selected as an optimum reaction parameters. Copyright © 2017 BCREC Group. All rights re-served
Keywords: Acetic Acid; Benzyl Alcohol; Esterification; Mesoporous; zeolite ZSM-5
How to Cite: Kusumaningtyas, D.T., Prasetyoko, D., Suprapto, Triwahyono, S., Jalil, A.A., Rosidah, A. (2017). Esterification of Benzyl Alcohol with Acetic Acid over Mesoporous H-ZSM-5. Bulletin of Chemi-cal Reaction Engineering & Catalysis, 12 (2): 243-250 (doi:10.9767/bcrec.12.2.806.243-250)
Available online at BCREC Website: http://bcrec.undip.ac.id
Zeolites are microporous crystalline alumi-nosilicate materials well known for their cata-lytic and adsorptive activity and selectivity. They also posses high surface area, high ther-mal and chemical stability and as such they have found application in a great number of processes ranging from petrochemical industry to environmental separations [1,2]. The activity
of zeolites is determined by their intrinsic acid-ity, of both Lewis and Brönsted nature, or by ac-tive species (mostly metal ions or oxides) that can be introduced into the zeolite structure. However, the sole microporosity of zeolites, which plays a crucial role in their shape selec-tivity, can also be their biggest drawback [3,4]. The different reaction in esterification of acetic acid with benzyl alcohol using catalysts of Hβ, HY, and H-ZSM-5 have also been observed . The research showed that in addition to acidity, pore zeolite plays a very important role in the catalytic activity of ZSM-5. Molecules with diameters larger than the framework pore * Corresponding Author.
Telp.: +6231-5943353; Fax.: +6231-5928314
Bulletin of Chemical Reaction Engineering & Catalysis, 12 (2), 2017, 244
openings are restricted from entering and approaching the active sites. This imposes sig-nificant limitations in terms of the range of reactions that can be efficiently catalyzed.
Introduction of mesoporous into originally microporous zeolitic structures is one approach to obtaining the best of both worlds, i.e. creating materials with lower diffusion restric-tions, which are able to host larger molecular species, while still retaining desired acidity of the active sites within the structure [4,5]. Such microporous/mesoporous zeolites are called hierarchical, a term which designates a zeolitic material with at least one additional level of porosity besides the intrinsic micropore system. The development of mesopority can be achieved by both synthetic and post-synthetic routes [6-8].
Hierarchical synthesis of ZSM-5 has been developed from kaolin as a source of silica and alumina, silicalite seed is added as to induced of ZSM-5 structure and CTABr for mesostruc-ture . Hierarchical ZSM-5 synthesized with temperature aging at 70 °C for 6, 12, and 24 hours. The results showed that the longer of aging time, the crystallinity of ZSM-5 was increased, but the area and volume of mesoporous tends to decrease. Furthermore, in this paper, we describe the correlation between acidity and crystallinity of mesoporous ZSM-5 synthesized from Bangka-Belitung’s kaolin.
In present study, the performance of H-ZSM-5 mesoporous was evaluated in benzy-lation of acetic acid (AA) with benzyl alcohol (BA). The effect of pore size of zeolite H-ZSM-5 mesoporous on the catalytic activity was inves-tigated. The detailed optimization of process parameters, such as: molar ratio and catalyst loading, were also carried out with aim to maximize AA conversion.
2. Materials and Methods 2.1. Materials
The raw material of kaolin were obtained from Bangka Belitung (Al4(Si4O10)(OH)8, 47 % SiO2 and 22 % Al2O3), sodium hydroxide (NaOH pellet, Merck, 99 %), LUDOX (SiO2, Al-drich, 30 %), and cetyltrimethylammoniumbro-mide (CTABr, C19H42BrN, Merck, 97 %), ammo-nium acetate (CH3COONH4, Merck, >98 %), benzyl alcohol (C6H5CH2OH, Merck, 99.5 %), acetic acid glacial (CH3COOH, 100 %), aqua demineralization (aqua DM), pyridine (C5H5N, Merck, 99.9 %), potassium hydroxide (KOH, pellet, 85 %), oxalic acid (H2C2O4, Merck, 99.5 %), ethanol (C2H6O, Merck, 99.9 %), n-hexane
(C6H14, Merck, 99 %), and phenolptalein indica-tor (C20H14O4, Merck).
2.2. Synthesis of catalysts
The mesoporous ZSM-5 has been synthe-sized . It has been synthesynthe-sized by hydrother-mal method with two stages of crystallization. The mesoporous ZSM-5 were synthesized in a starting aluminosilicate gel with the compo-nents of 10 Na2O : 100 SiO2 : 2 Al2O3 : 1800 H2O mol ratio with a various aging time, i.e 6, 12 and 24 h at 70 °C, namely: A-6-70, A-12-70 and A-24-70. In this study, the cationic surfac-tant was added for mesostructure and seed silicalite to induce MFI structure.
Na-ZSM-5 mesoporous was weighed as much as 1.0 gram then was inserted into the three-neck-flask size 250 mL, then, was added
by 50 mL ammonium acetate 1 M. Subsequently, the mixture located within the
round flask was connected with reflux and was heated to a temperature of 60 °C, stirred for 3 hours at a speed of 500 rpm. Once completed, the mixture was filtered in a round flask with filter paper to obtain a precipitate. The precipi-tate was roasted prior to dry and then calcined at 550 °C for 1 h in N2 and 6 h in air to obtain H-ZSM-5 [10,11]. Further, the catalysts were known as HZ-6, HZ-12, and HZ-24.
2.3. Catalyst Characterization
Bulletin of Chemical Reaction Engineering & Catalysis, 12 (2), 2017, 245
discs at room temperature. The adsorption was carried out at room temperature for 1 h. The desorption procedure were conducted at 150 °C for 3 h in order to determine the acidity of Lewis and Brönsted acid sites by evaluating the amount of remaining adsorbed pyridine as temperature increases . The concentrations of Brönsted (B) and Lewis (L) acid sites were calculated from the peak areas of adsorbed pyridine at around 1540 and 1450 cm−1, using B and L extinction coefficients (k) of 1.88 and 1.42 cm.mmol−1, respectively .
where, B = peak area of Lewis or Brönsted acid bond (cm-1); L = area of disk sample (cm2); and g = weigh of disk sample (g).
The scanning electron microscopy (SEM) images were obtained from SEM (ZEISS EVO MA 10). Dry samples were Pd/Au coated prior to scanning. Concentration of Si and Al were determined by means of energy dispersive spec-troscopy (EDX BRUKER 129 EV).
2.4. Catalytic performance
The synthesized catalysts were evaluated in benzylation of acetic acid with benzyl alcohol, which was carried out in a three-necked glass round bottom flask of 250 mL capacity equipped with a reflux condenser to prevent the escape of acetic acid, a thermometer and a magnetic stirrer. The flask was charged with acetic acid and benzyl alcohol both weighted sequentially, followed by the addition of the catalyst. Then, the system was heated up to desire temperature (383 K), the reaction was carried out for 3 h, and finally the product was collected after removing the catalyst. For deter-mination of free fatty acids conversion, 1 g sample was mixed with 5 mL of 96 % ethanol and 5 mL n-hexane. Then the 3 drops of phenolphthalein indicator was added and titrated with 0.1 N KOH solution. Previously, the KOH has been standardized with oxalic acid 0.1 N. The titration was stopped when the color of the solution changes to pink which can last up to 30 seconds.
3. Results and Discussion
3.1. Characterization of catalyst The XRD patterns (Figure 1) shows that all the investigated samples preserved their MFI structure. However, the aging time influence the degree of crystallinity in the mesoporous samples. The rate of crystallization by aging more quickly than without aging  and the aging process serves to increase the nucleation, reducing the induction time and crystallization . The variations in crystallinity of the mesoporous ZSM-5 (Table 1) was calculated based on the relative intensities of the reflec-tion at 2θ of 23°, taking the crystallinity of the ZSM-5 commercial to be 100 %.
The isotherms of the nitrogen adsorption-desorption of mesoporous samples are shown in 3 10 ) / ( w x k l x B g mmol acid of Amount sample weight Mr x N x V
FFA KOH KOH KOH
% final final initial FFA x FFA FFA Conv % % 100 % % %
Table 1. The content of intensity and crystallinity of the samples
Sample 2θ Intensity Crystallinity (%)
ZSM-5 commercial 23.14° 1813 100
A-6-70 23.04° 218.68 12.06
A-12-70 23.04° 423.44 23.36
A-24-70 23.04° 501.95 27.69
Bulletin of Chemical Reaction Engineering & Catalysis, 12 (2), 2017, 246
Figure 2. However, the mesoporous area, pore diameter, and mesoporous volume are shown in Table 2. All the isotherms showed type IV adsorption. As it can be seen from Table 2, the
SBET, Smeso and Vmeso decrease with increasing ZSM-5 crystallinity. This phenomenon indi-cates that the crystallization of ZSM-5 occurs in the core of the mesophase particles, so that amorphous silica that acts as an intermediate in the transformation of the mesoporous walls into ZSM-5, is precipitated on the ZSM-5 crys-tallites preventing the access of nitrogen into the pores .
The acidity was aimed to determine the amount of Lewis and Brönsted acid sites of the samples. Surface acidity analysis was per-formed using pyridine adsorption and was ana-lyzed by infrared spectroscopy. The Lewis and Brönsted acid sites can be known if there is a peak between 1440-1460 cm-1 and 1545-1600 cm-1. The acidity of the sample H-ZSM-5 mesoporous shown in Figure 3. All samples have Lewis acid sites (peak appears at wavenumber of 1442) and Brönsted acid sites
(peak appears at wavenumber of 1550). Table 3 shows the amount of the Lewis acid and Brön-sted acid sites of those samples. Lewis acid number of the A-6-70 samples is higher than others. The characterization by pyridine
ad-sorption showed that at the higher crystallinity, the number of Lewis acid and
Brönsted acid sites were decreased.
In this study, the A-12-70 catalyst has been selected to be observed its morphology and mapping (distribution) of the elements contained using instrument SEM-EDX. The observation of the surface of the catalyst is shown in Figures 4-5. In Figure 4 shows the morphology of the crystal-shaped beam. The results of SEM characterization were also obtained an average particle size of approxi-mately 1 µ (1000 nm). The distribution of the elements contained in the A-12-70 catalyst is shown in Figure 5. The Figure 5a shows that the elements of Na, Si, Al, and O were spread evenly on the catalyst and Figure 5b shows the EDX spectrum of catalyst.
Table 2. Textural properties of mesoporous ZSM-5 Figure 2. N2 adsorption-desorption Isotherm of
samples a. A-6-70, b. A-12-70, c. A-24-70 Figure 3. A-12-70, c. A-24-70 FTIR-Pyridine Spectra, a. A-6-70, b.
Sample SBET(m2/g) Smeso(m2/g) Vmeso (cm3/g) Dmeso (nm)
A-6-70 816.96 255.78 0.31 3.84
A-12-70 709.45 120.86 0.22 3.83
A-24-70 696.64 88.48 0.18 3.84
3 g -1)
Bulletin of Chemical Reaction Engineering & Catalysis, 12 (2), 2017, 247
Sample Surface area (m2/g) Crystallinity (%) acid sites (mmol/g) Amount of Lewis Amount of Brönsted acid sites (mmol/g)
A-6-70 255.78 12.06 0.27322 0.20612
A-12-70 120.86 23.36 0.19075 0.18898
A-24-70 88.48 27.69 0.08713 0.30956
Table 3. The amount of Lewis and Brønsted acid
Figure 5. Mapping of A-12-70 catalyst (a) and EDX spectrum of A-12-70 (b) Figure 4. A-12-70 morphology using SEM
Bulletin of Chemical Reaction Engineering & Catalysis, 12 (2), 2017, 248
3.2. Catalytic activity
3.2.1. Effect of catalyst properties on benzyla-tion
Initial experiments were carried at 383 K, 1:4 (AA to BA) molar ratio, catalyst loading of 5 % (wt.% of AA), and reaction time of 3 h. The HZ-6 was found to be potential catalyst with higher AA conversion of 37 % which is attributed to the high acidity and pore volume of 0.31 cm3.g-1 (Figure 6). Hence, the detailed optimization of process parameters was carried out for benzylation of AA with BA over HZ-6.
3.2.2. Influence of molar ratio
Benzylation of AA with BA was carried out by varying the molar ratio of AA to BA from 1:2 to 1:6 over HZ-6 to assess its effect on the cata-lytic activity. The effect of mole ratio over the conversion can be attributed with the occu-pancy of alcohols over the active sites and the
availability of acid molecules for further esteri-fication. The conversion of AA was found increase from 25 to 39 % with an increase in reactant molar ratio from 1:2 to 1:4 (Figure 7). The conversion of AA significantly decreases its molar ratio from 1:4 to 1:6. Although the increase in alcohol content might be expected to increase the conversion, there might be dilu-tion of acetic acid by increased alcohol contents, thereby preventing acetic acid adsorption on Brönsted acid sites . Thus, all the further reactions were performed with a molar ratio (AA:BA) of 1:4.
3.2.3. Influence of catalyst loading
The effect of catalyst loading on the reaction was evaluated by varying the catalyst from 2.5 to 10 % (wt.% of AA). The AA conversion was found increasing from 32 to 37 % with increase in catalyst loading from 2.5 to 5 % (Figure 8). Increasing conversion with increase in the catalyst amount is due to the availability of large surface area, which favors the dispersion of more active species. Therefore, accessibility of the large molecule of the reactant to the catalyst active site is favored . Further increase in catalyst loading, the AA conversion was found to be decreased. The 5 % catalyst loading was observed to be optimum with AA conversion of 37 %.
3.2. Mechanism for benzylation reaction The catalytic mechanism for synthesis of benzyl acetate by benzylation of AA with BA is proposed in Scheme 1. The reaction mechanism follows Fischer esterification involving several steps: starts with adsorption of AA on Brönsted acid sites present on the catalyst surface,
Figure 7. Influence of molar ratio on benzyla-tion AA with BA over HZ-6 at catalyst loading 10 %, reaction temperature of 383 K and reac-tion time of 3 h
Figure 8. Influence of catalyst loading on ben-zylation AA with BA over HZ-6 at molar ratio 1:4, reaction temperature of 383 K and reac-tion time of 3 h
Figure 6. Benzylation of AA with BA over HZ-6, HZ-12 and HZ-24 at molar ratio (AA:BA) of 1:4, catalyst loading of 5 %, reaction tempera-ture of 383 K and reaction time of 3 h
Bulletin of Chemical Reaction Engineering & Catalysis, 12 (2), 2017, 249
forming an intermediate of protonated AA, which increases the electrophilicity of carbonyl carbon [18,19]. The H-ZSM-5 mesoporous cata-lyst facilitates the protonation of the carbonyl oxygen atom, due to large pore volume, which eliminates steric hindrances among framework and substituted groups. Nucleophilic oxygen atom from BA attracts the carbonyl carbon which forms an oxonium ion. The transfer of proton in an oxonium ion leads to formation of a new oxonium ion, with the losing molecule of water from last oxonium ion and followed by deprotonation forms the benzyl acetate, with the regeneration acid site on the surface of catalyst (Scheme 1).
Mesoporous ZSM-5 has been successfully synthesized from kaolin Bangka Belitung and colloidal silicate as aluminum and silicon source. Characterization using XRD results showed that the degree of crystallinity decreases with increasing mesopority. Nitrogen adsorption-desorption results showed that the longer of aging time, the surface area, and
volume of mesoporous tends to decrease. Characterization by pyridine adsorption showed that the higher crystallinity, the num-ber of Lewis acid sites were decreased. The highest mesoporous surface area and Lewis acid sites was obtained by sample which have a lowest crystallinity, i.e. 255.78 m2/g and 0.2732 mmol/g, respectively. The benzylation of acetic acid (AA) with benzyl alcohol (BA) has been carried out over zeolites H-ZSM-5 (HZ-6, HZ-12 and HZ-24). The AA conversion was in the order of HZ-6 > HZ 12 > HZ-24. This mi-cro/meso-HZSM-5 can be regarded as promising heterogeneous acid catalyst to improve the selectivity of desired mono-benzylated product in aromatic benzylation and has potential application for chemical and pharmaceutical industry.
The authors would like to acknowledge the Ministry of Research and Higher Education, Indonesia, under “PUPT” research grant No. 003246.18/IT2.11/PN.08/2016.
Bulletin of Chemical Reaction Engineering & Catalysis, 12 (2), 2017, 250
 Vermeiren, W., Gilson, J.P. (2009). Impact of
Zeolites on the Petroleum and Petrochemical
Industry. Topics in Catalysis, 52: 1131-1161.
 Panagiotis, M. (2011). Application of Natural
Zeolites in Environmental Remediation: A
Short Review. Microporous Mesoporous
Mate-rial, 144: 15-18.
 van Donk, S., Janssen, A.H., Bitter, J.H., de
Jong, K.P. Generation, Characterization, and
Impact of Mesopores in Zeolite Catalyst.
Ca-talysis Reviews: Science and Engineering, 45:
 Egeblad, K., Christensen, C.H., Kustova, M.,
Christensen, C.H. (2008). Templating
Mesoporous Zeolites. Chemistry of Materials,
 Perez-Ramirez, J., Christensen, C.H.,
Ege-blad, K., Christensend, C.H., Groen, J.C. (2008). Hierarchical Zeolites: Enhanced Utili-sation of Microporous Crystals in Catalysis by
Advances in Materials Design. Chemical
Soci-ety Reviews, 37: 2530-2542.
 Xiao, F.S., Wang, L., Yin, C., Lin, K., Di, Y.,
Li, J., Xu, R., Su, D.S., Schlogl, R., Yokoi, T., Tatsumi, T. (2006). Catalytic Properties of Hi-erarchical Mesoporous Zeolites Templated with a Mixture of Small Organic Ammonium
Salts and Mesoscale Cationic Polymers.
Ange-wandte Chemie International Edition, 45:
 Zhao, J., Hua, Z., Liu, Z., Li, Y., Guo, L., Bu,
W., Cui, X., Ruan, M., Chen, H., Shi, J. (2009). Direct Fabrication of Mesoporous
Zeo-lite with a Hollow Capsular Structure.
Chemi-cal Communications, 48: 7578-7580.
 Chal, R., Cacciaguerra, T., van Donk, S.,
Gérardin, C. (2010). Pseudomorphic Synthesis
of Mesoporous Zeolite Y Crystals. Chemical
Communications, 46: 7840-7842
 Hamid, A. (2015). Synthesis of Mesoporous
ZSM-5 from Kaolin and Colloidal Silica with Two Step Crystallization : Influence of
Tem-perature and Aging Time. Master Thesis,
Ki-mia FMIPA, ITS Surabaya.
 Zein, Y.M. (2014). Biodiesel Production from Waste Palm Oil Catalyzed by Hierarchical
ZSM-5 Supported Calcium Oxide. Master
The-sis, Food Engineering and Bioprocess
Tech-nology, Asian Institute of Technology Thai-land.
 Bariyah, U. (2014). Pengaruh Rasio
SiO2/Al2O3 pada Sintesis ZSM-5 dan
Aktivi-tas Katalitiknya untuk Reaksi Esterifikasi.
Master Thesis, Kimia FMIPA, ITS Surabaya.
 Qoniah, I., Prasetyoko, D., Bahruji, H., Tri-wahyono, S., Jalil, A.A., Suprapto, Hartati, Purbaningtyas, T.E. (2015). Direct Synthesis of Mesoporous Aluminosilicates from
Indone-sian Kaolin Clay without Calcinations.
Ap-plied Clay Science 118: 290-294.
 Emeis, C.A. (1993). Determination of Inte-grated Molar Extinction Coefficients for In-frared Absorption Bands of Pyridine
Ad-sorbed on Solid Acid Catalysts. Journal of
Catalysis, 141: 347-354.
 Zhang, X., Wang, J., Liu, H., Liu, C., Yeung, K. (2003). Factors Affecting the Synthesis of Hetero-atom Zeolite FeZSM-5 Membrane.
Separation and Purification Technology, 32:
 Jihong, Y. (2007). Chapter 3 Synthesis of Zeo-lites. In: Čejka, Jiří, v. B., H., C., A., Ferdi, S.
(Eds.). Studies in Surface Science and
Cataly-sis. 168: 39-103.
 Goncalves, M.L., Dimitrov, L.D., Wallau, M., Urquieta-Gonzalez, E.A. (2006). Mesoporous ZSM-5 Synthesized by Simultaneous Mesostructuring and Crystallization of
ZSM-5 Nuclei. Scientific Bases for the Preparation
of Heterogeneous Catalysts, E.M. Gaigneaux
et al. (Editors), Elsevier, 323-330.
 Gokulakrishnan, N., Pandurangan, A., Sinha, P.K. (2007). Esterification of Acetic Acid with Propanol Isomers under Autogeneous Pres-sure : A Catalytic Study of Al-MCM-41
Mo-lecular Sieves. Journal of Molecular Catalysis
A: Chemical, 263: 55-61.
 Kirumakki, S.R., Nagaraju, N., Narayanan, S. (2004). A Comparative Esterification of Benzyl Alcohol with Acetic Acid over Zeolites
Hβ, HY, and HZSM-5. Applied Catalysis A:
General, 273: 1-9.
 Sawant, D.P., Vinu, A., Justus, J., Srinivasu, P., Halligudi, S.B. (2007). Catalytic Perform-ances of Silicotungstic Acid/Zirconia Sup-ported SBA-15 in an Esterification of Benzyl
Alcohol with Acetic Acid. Journal of
Molecu-lar Catalysis A : Chemical, 276: 150-157
Selected and Revised Papers from The 2nd International Seminar on Chemistry (ISoC 2016) (Surabaya, 26-27 July 2016) (http://chem.its.ac.id/isoc-2016/) after Peer-reviewed by Scientific Committee of ISoC 2016 and